Pré-visualização4 páginas

SFT. Table 2. Swirling chamber dimensions. Fig. 6. Influence of SC parameters on velocity distribution. Fig. 7. Path lines of flow fields in (a) one-strand SFT, (b) tundish with TI, (c) two-strand SFT. kg/m3 for the inclusion density of 3 000 kg/m3 in real condi- tion according to the similarity criterion (Eq. (9)). In fact, a similarity criterion can be obtained by dimen- sional analysis. Taking kinematical viscosity m , density r , the difference of density (r l�r inc), radius r, relative veloc- ity u and gravitational acceleration g into consideration, three dimensionless groups can be formed, Re�1, Fr�1 and (r l�r s)/r l. According to Buckingham’s P Theorem, the group of ReFr�1(r l�r s)/r l is actually the same as the analysis result from Sahai and Emi. 3.6. Trajectories of Inclusion Particles Different densities of inclusion were used in the litera- tures, e.g. 3 500 kg/m3 for spherical particles and 5 000 kg/m3 for clusters,16) 2 700 kg/m3 for spherical inclusions.15) Three densities are considered in this work for mathemati- cal model simulation (400, 500, 600 kg/m3) to examine the influence of density on separation ratio of inclusion. To calculate inclusion separation ratio, the injection of particles is set. The original injection position is on the inlet surface. The injected particles are set with different diame- ters and densities. 2 000 particles are released each time and their trajectories are calculated out with discrete ran- dom walk model. Each injection condition is repeated five times and then the total separation ratios are calculated. Twenty representative trajectories of inclusion particles in one-strand SFT, a tundish with TI and two-strand SFT are shown in Fig. 8. It can be seen that the trajectories for the same kind of inclusion particle are different. In the tundish with SC, most particles have longer trajectories in the im- pact zone than those in the tundish with TI. This can en- hance the removal of inclusion to slag–steel interface. Moreover, in the zone above the outlet, it can be seen that inclusion particles in the tundish with TI have greater pos- sibility to go into mold than those in the tundish with SC. From Fig. 8(c), one can see that the trajectories above the outlet are different for the left and right zones to the SC. The position of SC should thus be optimized for uniform quality of casting steel out of each outlet. 3.7. Comparison of Removal Possibility The influence of particle density on separation ratio is given in Fig. 9. It can be seen that the difference of density has a minor influence on separation ratio within the density range of 400–600 kg/m3. Moreover, according to the weight of inclusion distribution (shown in Fig. 10) from experi- mental samples, particles larger than 75 mm have little sig- nificance and can be neglected during simulation process. For larger diameters of particle (50 mm), the separation ratio of tundish with TI is higher than that of SFT. The rea- son for this is the short distance between the dam and the first weir or between dam and SC which can be seen from the trajectories shown in Figs. 11(a), 11(b). Because of these narrow spaces, the upward flow is very quick and it can be reflected instantly downward. Consequently, the en- trainment possibility of inclusion particles to slag–steel in- terface is decreased for inclusion particles. The SFT has been revised to alleviate this phenomenon. Both of the dis- tances between the dam and the first weir and between the weir and SC have been extended 100 mm in one simulation. It can be seen from Fig. 11(c) that the strong upward flow is weakened. As a result, the separation ratios of inclusions are improved as shown in Table 3, particularly for the 20 mm diameter particles. It should be pointed out here that the original positions of flow control devices were optimized for tundish with TI. However, the results show that they are no more suitable for SFT. For different design of flow control schemes, their po- sitions should be relocated for optimum operation. ISIJ International, Vol. 48 (2008), No. 6 791 © 2008 ISIJ Fig. 9. Relationships between removal ratio and density of inclu- sion particles. Fig. 10. Size distribution of inclusion in weight extracted from steel by Slimes method.17) Fig. 8. Trajectories of particles in tundishes: (a) one-strand SFT (H4, D3, Q1, 20 mm, 500 kg/m3), (b) TI (H4, D3, Q1, 20 mm, 500 kg/m3), (c) two-strand tundish with different particle diameters (Q2, H3, D2, 3 000 kg/m 3). 4. Conclusion A new swirling flow tundish has been developed and modelled by physical and mathematical methods. The nu- merical model is validated by RTD and flow field respec- tively. The flow fields, the motion and separation of inclu- sions are examined too. The conclusion can be drawn as follow. (1) Flow fields in SFT are asymmetrical for both one- strand and two-strand. Because of the introduction of SC, the inlet is not set in a symmetrical position as usual. Hence, the whole flow field is changed to be more compli- cated and not symmetrical. (2) Inclusions have more chance of flotation to slag– steel interface in SFT than the tundish with TI. The separa- tion ratios show that SFT have greater ability to remove in- clusion than the tundish with TI. Especially for small parti- cle, for example 20 mm, SFT’s advantage is evident. This is especially important for producing high quality steel. (3) For different designs of tundish, the positions of all flow control devices and SC should be relocated for opti- mum metallurgical effects. Acknowledgement One of the authors (Q. F. Hou) would like to make grate- ful acknowledgements to the Centre for Simulation and Modelling of Particulate Systems (SIMPAS) for the visiting fellowship. Nomenclature C : Concentration of tracer (kg/m3) De : Effective turbulent mass diffusivity (m 2/s) Dsc : Diameter of swirling chamber (mm) H : Height of tundish (mm) Hsc : Height of swirling chamber (mm) k : Turbulent kinetic energy (J/kg) L1 : Top length of tundish (mm) L2 : Bottom length of tundish (mm) P : Pressure (Pa) Q : Inlet flowrate (Nm3/h) R : Radius of inclusion Rt : Rotational similarity criterion ui : Velocity in the xi direction (m/s) W1 : Top width of tundish (mm) W2 : Bottom width of tundish (mm) xi : Cartesian coordinates vector F : Inlet diameter (mm) e : Dissipation rate of kinetic energy (m2/s3) r : Density (kg/m3) m : Molecular viscosity of fluid (Pa · s) m t : Turbulent viscosity of fluid (Pa · s) m eff : Effective viscosity of fluid (Pa · s) w : Rotational speed (rpm) Subscript inc : Inclusion m : Model p : Prototype st : Steel w : Water REFERENCES 1) L. F. Zhang and B. G. Thomas: ISIJ Int., 43 (2003), 271. 2) D. Mazumdar and R. I. L. Guthrie: ISIJ Int., 39 (1999), 524. 3) J. D. J. Barreto-Sandoval, A. W. D. Hills, M. A. Barron-Meza and R. D. Morales: ISIJ Int., 36 (1996), 1174. 4) A. Ramos-Banderas, R. D. Morales, L. Garcia-Demedices and M. Diaz-Cruz: ISIJ Int., 43 (2003), 653. 5) Y. Miki, S. Ogura and T. Fujii: Kawasaki Steel Tech. Rep., (1996), 67. 6) Z. Zou, Q. Hou, S. Kuang and H. Li: SCANMET II—2nd Int. Conf. on Process, MEFOS, Luleå, Sweden, (2004). 7) F. Wang, B. Li and F. Tsukihashi: ISIJ Int., 47 (2007), 568. 8) Q. F. Hou and Z. S. Zou: Kang T’ieh/Iron Steel (Peking), 40 (2005), 33. 9) Q. Hou and Z. Zou: ISIJ Int., 45 (2005), 325. 10) Q. Hou and Z. Zou: Steel Res. Int., 76 (2005), 726. 11) Y. Murakata, M. G. Sung, K. Sassa and S. Asai: Tetsu-to-Hagané, 92 (2006), 579. 12) V. Chevrier and A. W. Cramb: Scand. J. Metall., 34 (2005), 89. 13) K. Beskow, J. Jia, C. H. P. Lupis and S. C. Du: Ironmaking Steelmak- ing, 29 (2002), 427. 14) A. Haider and O. Levenspiel: Powder Technol., 58 (1989), 63. 15) A. K. Sinha and Y. Sahai: ISIJ Int., 33 (1993), 556. 16) S. Lopez-Ramirez, J. D. J. Barreto, J. Palafox-Ramos, R. D. Morales and D. Zacharias: Metall. Mater. Trans. B, 32B (2001), 615. 17) L. F. Zhang, S. Taniguchi and K. K. Cai: Metall. Mater. Trans. B, 31B (2000), 253. 18)